Abstract
Temperaturedependent electrical characterization of Pt/nGaN Schottky barrier diodes prepared by ultra high vacuum evaporation has been done. Analysis has been made to determine the origin of the anomalous temperature dependence of the Schottky barrier height, the ideality factor, and the Richardson constant calculated from the IVT characteristics. Variabletemperature Hall effect measurements have been carried out to understand charge transport at low temperature. The modified activation energy plot from the barrier inhomogeneity model has given the value of 32.2 A/(cm^{2} K^{2}) for the Richardson constant A** in the temperature range 200 to 380 K which is close to the known value of 26.4A/(cm^{2} K^{2}) for ntype GaN.
Background
GaN has been the subject of strategic research among all compound semiconductors and has been explored widely and rightly for its various characteristics, like direct wide band gap, high breakdown field, high saturation velocity, and chemical and radiation hardness [1]. The combination of all these properties makes GaN a preferred material for optoelectronics and hightemperature and highpower RF applications. In applications like power rectifier and HEMT, a metal–semiconductor contact with high Schottky barrier height (SBH), high rectification efficiency, and low reverse leakage current is needed [1,2]. Also, the quality of the metal–semiconductor interface is affected by the process steps and deposition vacuum since contamination and oxide layer growth at the interface may result in SBH reduction and high leakage current by inducing local nanoscopic patches of low barrier heights. Werner and Güttler reported that these local patches follow a Gaussian distribution of barrier height and locally control the device characteristics in different temperature regimes of operation [3]. Studies by Tung revealed that this kind of inhomogeneous behavior is observed in all semiconductors and results in overall decreased barrier heights [4]. The contamination level and oxide layer can be minimized by following fabrication steps in a clean room and depositing Schottky metals in ultra high vacuum (UHV). According to the SchottkyMott model, the Schottky barrier height is dependent on the metal work function and electron affinity of semiconductor χ (GaN χ = 4.1 eV) [1,5,6]. Metals like Pt, Ni, Pd, and Au which have high work function than GaN make a better choice for gate contact. Pt has a high work function (5.65 eV) that makes it ideal for use as Schottky contacts on ntype GaN, and it is also resistant to oxidation and corrosion [1]. There are only a few reports on Pt/GaN Schottky barrier diodes. The Schottky barrier height of Pt/nGaN has been reported with a value between 0.89 and 1.27 eV [712]. In the present paper, we report an investigation on goodquality Pt/GaN Schottky barrier diodes deposited in ultra high vacuum condition. Temperaturedependent IV characteristics have been measured and analyzed using the barrier inhomogeneity model proposed by Werner and Güttler [3].
Methods
GaN epitaxial layers used in this study were grown on a cplane sapphire substrate by metal organic chemical vapor deposition (MOCVD). The GaN epitaxial layers were 3.4 μm thick and unintentionally doped (N_{D}^{+} approximately 3 × 10^{16} cm^{3} by Hall measurements). For Pt/nGaN diodes fabricated with indium ohmic contacts on nGaN epilayers, first the sample was cleaned sequentially with (1) methylpropanol (MP) at around 80°C for 8 min, (2) deionized (DI)water dip, (3) acetone at 50°C for 7 min, (4) isopropanol in ultrasonic bath for 3 min, and again a (5) DI water rinse and dry nitrogen blowing for drying the sample. After that contact, metallization was done by lithography/liftoff techniques. Photoresist (AZ5214), developer (AZ 400 K/H_{2}O 1:4), and native oxide layer removal (50% HCl for 1 min, rinse in H_{2}O) were applied. Then the sample was immediately transferred to an UHV deposition facility (base pressure in the vacuum chamber was 10^{10} mbar) for Pt/Au (100/100 nm) Schottky contact deposition. All these steps were carried out in a Class 100 cleanroom facility. Indium (In) ohmic contacts were deposited at two opposite edges by soldering in  second step. The schematic view of the Schottky barrier diodes fabricated in this work is shown in Figure 1. The current–voltage (IV) characteristics of the devices were measured using a programmable Keithley SourceMeter (model 2400, Keithley Instruments, Inc., Cleveland, OH, USA) in the temperature range 100 to 380 K with a temperature step of 40 K in an LN_{2} cryostat. Temperaturedependent Hall and resistivity measurements on GaN epitaxial layer were performed using a variabletemperature Hall setup from Ecopia Corporation, Anyangsi, South Korea (model HMS 5300).
Figure 1. Schematic diagram of the Pt/nGaN Schottky barrier diode fabricated on nGaN epitaxial layers.
Results and discussion
Before the fabrication of metal/nGaN contacts, structural and morphological characterizations of epitaxial layers have been done. The Xray diffraction pattern of the GaN epitaxial layer using CuKα radiation is shown below in Figure 2a. The Xray diffraction pattern was taken in bulk mode. The orientation of the epitaxial layer was observed to be along the (002) which confirms the growth of the epitaxial layer along the [0001] direction having a hexagonal (wurtzite) crystal structure. Additional diffraction peaks from (102), (004), and (203) reflection planes of hexagonal GaN were also observed. The sharp diffraction peaks (FWHM value 432 arc sec for (002)) reveal the reasonably good crystalline quality of the GaN epitaxial layer [13]. The lattice constants ‘a’ and ‘c’ were found to be 0.320 and 0.518 nm, respectively, which matched well with the standard cell parameter values as given in JCPDS card 02–1078. GaN epitaxial layers were also examined under an atomic force microscope (AFM) in the contact mode to measure the topography of the surface. Figure 2b shows the AFM images in a 2D view for the pristine samples. The surface area scanned was 10 × 10 μm^{2}. The RMS roughness of the surfaces is around 1 nm for all samples. The result of the AFM measurement shows an overall smooth GaN surfaces. These samples have an average dislocation density value of about 5 × 10^{8} cm^{2}, which is acceptable for GaN epilayers but poor as compared to Si and GaAs epilayers.
Figure 2. Xray diffraction spectrum (a) and AFM image (b) of the GaN epitaxial layer. The asterisk ‘*’ indicates peaks from sapphire substrate.
Electrical characterization of Schottky barrier devices was carried out in the temperature range of 100 to 340 K measured at a temperature interval of 40 K. Figure 3 shows the experimental semilog forward and reverse bias IV characteristics of the Pt/nGaN Schottky barrier diodes (SBD). It should be mentioned here that for analysis, we have used diodes with 384μm diameter and have almost identical electrical properties. The characteristics shown here demonstrate an average trend which was determined for a group of diodes. The current–voltage characteristics of SBD are given by the thermionic emission theory [14,15]. For bias voltage V ≥ 3kT/q, the conventional diode equation is
Figure 3. Semilog forward and reverse IV characteristics for Pt/nGaN Schottky diode at 100 to 340 K.
Here, A** is the effective Richardson constant, ϕ_{ap} is the apparent or measured barrier height, n is the ideality parameter, A is the diode area, and the other symbols have their usual meanings. Since image force is a very weak function of applied voltage, it could also be neglected [1418]. The experimental IV data is plotted as log I versus V and SBH, and n is calculated from the intercept and slope of the linear fit to the linear part of forward characteristics as given by Equations 2 and 3:
The measured ϕ_{ap}, n, and reverse leakage current (I_{R} at 1 V) are listed in Table 1. The Schottky barrier height and the ideality factor of the Pt contact are 1.03 eV and 1.38, respectively. The experimental values of SBH (ϕ_{ap}) and n vary from 1.1 eV and 1.25 (340 K) to 0.31 eV and 3.40 (100 K), respectively. The value of room temperature (300 K) SBH and n are 1.03 eV and 1.48, respectively. The measured SBH value of 1.03 eV for the Pt/nGaN at 300 K is lower than the ideal value of 1.54 eV, calculated according to the SchottkyMott model. High series resistance was found approximately 10 kΩ at RT, as calculated by the Cheung and Cheung method [19]. The SBH (ϕ_{ap}) and ideality factor versus temperature plots are given in Figure 4. The SBH decreases and the ideality factor increases with decrease in temperature. Temperature dependence of the measured SBH from the forward bias IV is usually explained in terms of the temperature dependence of the semiconductor band gap. However, in ‘real’ Schottky diodes, it is commonly observed that the temperature coefficient of the SBH differs substantially from the bandgap temperature coefficient and is often of the opposite sign. Such a temperature dependence of both the SBH and ideality factor n has often been accredited to current transport mechanisms not following the ideal thermionic emission theory. Various studies have cited different reasons for this nonideal dependence. Werner and Güttler [3] proposed that such dependence originates from Schottky barrier inhomogeneity, which could be due to different interface qualities. The quality of the interface depends on several factors such as surface defect density, surface treatment (cleaning, etching, etc.), deposition processes (evaporation, sputtering, etc.), and local enhancement of electric field which can also yield a local reduction of the SBH [3,16,17,2022]. This leads to inhomogeneities in the transport current [3,16,17,2022].
Table 1. Calculated Schottky diode parameters for Pt/nGaN Schottky diodes
Figure 4. Apparent SBH and ideality factor versus temperature plots for the Pt/nGaN Schottky diode.
The barrier inhomogeneity model assumes a continuous spatial distribution of the local Schottky barrier patches. The shape and position of the ridges in the potential ‘mountains’ depend on bias voltage and cause, therefore, idealities n > 1 in IV curves. The total current across a Schottky diode is obtained by integrating the thermionic current expression with an individual SBH and weighted using the Gaussian distribution function across all patches. This approach, however, does not consider the lateral length scale of the inhomogeneity and the pinchoff effect related to the interaction between adjacent regions with different SBHs. The approach points out that the apparent SBH is always lower than the mean value of the barrier distribution and is given with the following expression [3,17,18,23]:
where ϕ_{ap} is the apparent SBH measured from the forward bias IV characteristics and σ_{so} is the zerobias standard deviation of the SBH distribution and a measure of the barrier homogeneity. The temperature dependence of σ_{so} is usually small and can be neglected. Thus, SBH has a Gaussian distribution with the zerobias mean SBH, ϕ_{bo}. The variation in ideality factor n with temperature in the model is given by [3,17,24]
The voltageindependent ideality factor n requires a linear increase in ϕ_{b}(V, T) with the bias. This is only possible if the mean SBH ϕ_{b} as well as the square of the standard deviation σ^{2} varies linearly with the bias [3,17,18,24]:
As can be seen from Equations 6 and 7, ρ_{2} is the voltage coefficient of the mean SBH, and ρ_{3} is the voltage coefficient of the standard deviation. According to Equation 5, a plot of (n^{1} 1) against 1/T should give a straight line with the slope and yaxis intercept related to the voltage coefficients ρ_{2} and ρ_{3}, respectively. The value of ρ_{3} indicates that the distribution of the SBH becomes more homogeneous with voltage increase. A linear ϕ_{ap} versus 1/T curve means that the plot obeys the barrier inhomogeneity model. The experimental (n^{1} 1) and ϕ_{ap} versus 1/T plots in Figure 5 correspond to two lines instead of a single straight line with transition occurring at 200 K. The values of ρ_{2} obtained from the intercepts of the experimental (n^{1}  1) versus 1/T plot are shown in Figure 5. The intercept and slope of the straight line have given two sets of values of ϕ_{bo} and σ_{so} in the temperature range of 100 to 180 K and in the temperature range of 220 to 340 K, respectively. Our results are similar to the results obtained for Pd/nGaN and Pt/nGaN in the temperature range of 80 to 400 K [25].
Figure 5. Zerobias apparent barrier height (stars) and ideality factor function (n^{1}  1) versus 1/(2kT) (filled boxes) curves.
Further, the conventional saturation current expression can be written for the activation energy plot or Richardson plot by rewriting Equation 2 as follows:
The conventional activation energy ln(I_{0}/T^{2}) versus 1/T plot should be linear in ideal case and gives A** and SBH as intercept and slope calculations based on the TE current mechanism. For inhomogeneous diodes, this is not true. Therefore, a modified activation energy expression according to the Gaussian distribution of the SBHs can be rewritten by incorporating Equations 4 and 5 in Equation 8:
Using the experimental I_{0} data, the modified activation energy plot or Richardson plot (
Figure 6. Modified Richardson plot, [ln(I_{0}/T^{2})  q^{2}σ_{so}^{2}/2k^{2}T^{2}] versus 1/T, for the Pt/nGaN Schottky diode.
To physically understand the origin of this barrier inhomogeneity in two different
temperature regimes and to comprehend the current transport at low temperatures, we
performed variabletemperature Hall measurements. In Figure 7, the N_{D}^{+} (carrier concentration) values measured from Hall measurements are shown for the
temperature range of 80 to 350 K for ntype GaN samples. It is well known that N_{C} for ntype GaN samples is
Figure 7. Carrier concentration (N_{D}^{+}), resistivity (ρ), and mobility (μ) as a function of temperature for nGaN.
Conclusions
In conclusion, a detailed electrical analysis of the Pt/nGaN Schottky contacts prepared by evaporation has been made to determine the origin of the anomalous temperature dependence of the SBH, the ideality factor, and the Richardson constant calculated from the IVT characteristics. The variabletemperature Hall experiments have given an insight into the origin of barrier inhomogeneity observed commonly in nGaNbased Schottky barrier diodes. The temperature dependence of the experimental values of SBH of the Pt/nGaN has been described by two Gaussian distributions in the temperature range of 100 to 340 K. The modified activation energy plot from the barrier inhomogeneity model has given the value of 32.2 A/(cm^{2} K^{2}) for the Richardson constant A** in the temperature range 200 to 380 K which is close to the known value of 26.4 A/(cm^{2} K^{2}) for ntype GaN.
Competing interests
The authors declare that they have no competing interests.
Authors’ contributions
AK carried out the research, drafted this manuscript. SA contributed in device fabrication. MCA is the research collaborator who provided experimental facilities. RS is PhD supervisor of AK. The manuscript was sent to all contributors. All authors read and approved the final manuscript.
Acknowledgements
Ashish Kumar would like to gratefully acknowledge the University Grant Commission (UGC) for providing research fellowship. We are thankful to Dr. Seema Vinayak from Solid State Physical Laboratory (SSPL), Delhi, India, for providing help in the experiments.
References

Morkoç H: Handbook of Nitride Semiconductors and Devices. Wiley: Weinheim; 2008.

Li S, Ware M, Wu J, Minor P, Wang Z, Wu Z, Jiang Y, Salamo GJ, Li S, Ware M, Wu J, Minor P, Wang Z, Wu Z, Jiang Y, Salamo GJ: Polarization induced pnjunction without dopant in graded AlGaN coherently strained on GaN.
Appl Phys Lett 2012, 101:1221031221033. Publisher Full Text

Werner JH, Güttler HH: Barrier inhomogeneities at Schottky contacts.
J Appl Phys 1991, 69:15221533. Publisher Full Text

Tung RT: Recent advances in Schottky barrier concepts.
Mater Sci Eng R Rep 2001, 35:1138. Publisher Full Text

Sze SM, Ng KK: Physics of Semiconductor Devices. Hoboken: Wiley; 2007.

Rhoderick EH, Williams RH: Metal–semiconductor Contacts. Oxford/New York: Oxford University Press/Clarendon Press; 1988.

Leung BH, Chan NH, Fong WK, Zhu CF, Ng SW, Lui HF, Tong KY, Surya C, Lu LW, Ge WK: Characterization of deep levels in PtGaN Schottky diodes deposited on intermediatetemperature buffer layers.
IEEE T Electron Dev 2002, 49:314318. Publisher Full Text

Iucolano F, Roccaforte F, Giannazzo F, Raineri V: Temperature behavior of inhomogeneous Pt/GaN Schottky contacts.
Appl Phys Lett 2007, 90:0921190921193. Publisher Full Text

Ravinandan M, Rao PK, Reddy VR: Temperature dependence of current–voltage (IV) characteristics of Pt/Au Schottky contacts on ntype GaN.

Iucolano F, Roccaforte F, Giannazzo F, Raineri V: Barrier inhomogeneity and electrical properties of Pt/GaN Schottky contacts.
J Appl Phys 2007, 102:1137011137018. Publisher Full Text

Giannazzo F, Roccaforte F, Iucolano F, Raineri V, Ruffino F, Grimaldi MG: Nanoscale current transport through Schottky contacts on wide bandgap semiconductors.
J Vac Sci Technol B 2009, 27:789794. Publisher Full Text

Mohammad SN, Fan Z, Botchkarev AE, Kim W, Aktas O, Salvador A, Morkoc H: Nearideal platinumGaN Schottky diodes.
Electron Lett 1996, 32:598599. Publisher Full Text

Jeong JK, Kim HJ, Seo HC, Kim HJ, Yoon E, Hwang CS, Kim HJ: Improvement in the crystalline quality of epitaxial GaN films grown by MOCVD by adopting porous 4HSiC substrate.
Electrochem Solid St 2004, 7:C43C45. Publisher Full Text

Rhoderick EH: Metal–semiconductor contacts.
IEEE ProcI 1982, 129:114. Publisher Full Text

Sze SM: Citation classic  physics of semiconductordevices.

Arehart AR, Moran B, Speck JS, Mishra UK, DenBaars SP, Ringel SA: Effect of threading dislocation density on Ni/nGaN Schottky diode IV characteristics.
J Appl Phys 2006, 100:0237090237098. Publisher Full Text

Yildirim N, Ejderha K, Turut A: On temperaturedependent experimental IV and CV data of Ni/nGaN Schottky contacts.
J Appl Phys 2010, 108:1145061145068. Publisher Full Text

Dogan S, Duman S, Gurbulak B, Tuzemen S, Morkoc H: Temperature variation of current–voltage characteristics of Au/Ni/nGaN Schottky diodes.
Phys E 2009, 41:646651. Publisher Full Text

Cheung SK, Cheung NW: Extraction of Schottky diode parameters from forward current–voltage characteristics.
Appl Phys Lett 1986, 49:8587. Publisher Full Text

Arulkumaran S, Egawa T, Ishikawa H, Umeno M, Jimbo T: Effects of annealing on Ti, Pd, and Ni/nA1(0).Ga11(0).N89 Schottky diodes.
IEEE T Electron Dev 2001, 48:573580. Publisher Full Text

Zhou Y, Wang D, Ahyi C, Tin CC, Williams J, Park M, Williams NM, Hanser A, Preble EA: Temperaturedependent electrical characteristics of bulk GaN Schottky rectifier.
J Appl Phys 2007, 101:0245060245064. Publisher Full Text

Kalinina EV, Kuznetsov NI, Dmitriev VA, Irvine KG, Carter CH: Schottky barriers on nGaN grown on SiC.
J Electron Mater 1996, 25:831834. Publisher Full Text

Song YP, Vanmeirhaeghe RL, Laflere WH, Cardon F: On the difference in apparent barrier height as obtained from capacitancevoltage and current–voltagetemperature measurements on Al/PInp Schottky barriers.
Solid State Electron 1986, 29:633638. Publisher Full Text

Yildirim N, Turut A: A theoretical analysis together with experimental data of inhomogeneous Schottky barrier diodes.
Microelectron Eng 2009, 86:22702274. Publisher Full Text

Mamor M: Interface gap states and Schottky barrier inhomogeneity at metal/ntype GaN Schottky contacts.
J PhysCondens Mat 2009, 21:335802. Publisher Full Text

Lin YJ: Origins of the temperature dependence of the series resistance, ideality factor and barrier height based on the thermionic emission model for ntype GaN Schottky diodes.
Thin Solid Films 2010, 519:829832. Publisher Full Text